1. THERMAL, MECHANICAL AND MORPHOLOGICAL PROPERTIES OF POLYLACTIDE
TOUGHENED WITH P[CL-CO-LA] COPOLYESTERS AS BIODEGRADABLE IMPACT MODIFIERS
Jérémy Odent1, Jean-Marie Raquez1, Philippe Leclère2, Philippe Dubois1
1Laboratory of Polymeric and Composite Materials (LPCM) ; 2Laboratory for Chemistry of Novel Materials (CMN),
Center of Innovation and Research in Materials & Polymers (CIRMAP), University of Mons (UMONS), 23 Place du Parc, B-7000 Mons, Belgium
Contact : email@example.com
This work was supported by the European Commission and Région Wallonne FEDER program
(Materia Nova) and OPTI²MAT program of excellence, by the Interuniversity Attraction Pole program
of the Belgian Federal Science Policy Office (PAI 6/27) and by FNRS-FRFC. J. Odent thanks F.R.I.A.
for its financial support thesis grant. J.-M. Raquez is ‘‘chargé de recherche’’ and Ph. Leclère is
‘‘chercheur qualifié’’ by the F.R.S.-FNRS.
Due to its renewability, polylactide (PLA) is the most extensively researched and utilized biopolymer as substitute to conventional petroleum-based polymers in different applications such as
in automotive and electronic industries. However, the applications of PLA are currently limited by its brittle nature , and impact modifiers are generally required to enhance its impact
strength . However, most of commercially available impact modifiers specifically designed for PLA are made of ethylene-based copolymers, and therefore are not biodegradable. In this
study, poly(ε-caprolactone-co-D,L-lactide) (P[CL-co-LA]) random copolyesters were synthesized and investigated as novel biodegradable impact modifiers for PLA. The effect of the
molecular parameters of these as-synthesized copolyesters was investigated on the impact performance of PLA-based materials. The thermal, mechanical and morphological properties of
the blends proved highly dependent on the morphology and average size of the rubbery microdomains dispersed throughout the PLA matrix.
It appears that the use of a P[CL-co-LA] copolyester with a molar composition of 72/28 mol% (CL/LA) gives significant improvement in the impact strength by a factor of ca. 4.2 (E.I. = 11.4
kJ/m²) with respect to neat PLA. In this regard, it came out that the comonomer content of the P[CL-co-LA] copolyesters has an effect on the resulting morphologies of PLA/P[CL-co-LA]
blends, together with a significant improvement in toughness. Moreover, improvement in toughness more likely comes from the blend morphology and can be correlated to the shape and
average size (and related size-distribution) of the rubbery microdomains.
Synthesis of poly(ε-caprolactone-co-D,L-lactide) copolyesters
The random copolymerization was carried out by ring-opening polymerization (ROP) of ε-
caprolactone (CL) and D,L-lactide (LA) promoted by n-heptanol (ROH) and Sn(Oct)2 (for
initial [ROH]/[Sn(Oct)2] and ([CL]+[LA])/ROH] molar ratios of 100 and 200, respectively) at
160°C for 24h in bulk (scheme 1).
a) As determined by 1H NMR.
b) As determined by SEC (THF + 2% NEt3) via a relative calibration with PS standards.
c) As determined by gravimetry.
d) As determined by DSC (under N2 flow, heating rate of 10°C/min, second scan).
Table 1 shows that random P[CL-co-LA] copolyesters exhibit a glass transition temperature
below room temperature and no melting temperature for experimental molar LA
compositions higher than 28 mol%, representing an interesting feature for their use as
(rubbery-like) impact modifiers .
Scheme 1. Copolymerization of ε-caprolactone (CL) and D,L-lactide (LA) promoted by n-heptanol and Sn(Oct)2.
(g/mol) PDI b
1 91 / 9 34,700 2.2 98 -52 46 41
2 81 / 19 35,200 2.1 98 -47 33 0.9
3 72 / 28 33,900 2.1 99 -37 /// ///
4 62 / 38 32,500 2.1 99 -25 /// ///
5 51 / 49 31,500 2.1 99 -13 /// ///
Table 1. Molecular and thermal characteristics of random P[CL-co-LA] copolyesters with
various monomers feed ratios as obtained by ROP of CL with LA using Sn(Oct)2/n-heptanol.
 Rasal, R.M.; Janorkar, A.V.; Hirt, D.E.; Prog Polym Sci. 35(3) 338-356 (2010)
 Anderson, K.S.; Schreck, K.M.; Hillmyer, M.A.; Polym Rev. 48(1) 85-108 (2008)
 Ishida, S.; Nagasaki, R.; J Appl Polym Sci., 113(1) 558-566 (2009)
 Bucknall, C.B.; J Polym Sci, Part B: Polym Phys. 45(12) 1399-1409 (2007)
 Cho, K.; Yang, J.; Yoon, S., J Appl Polym Sci., 95(3) 748-755 (2005)
Results and Discussion
Melt-blending of PLA with random copolyesters
10 wt% P[CL-co-LA] copolyesters were dispersed by melt-blending within PLA using a DSM
twin-screw micro-compounder (Figure 1) at 200°C and 60 rpm for 3 min followed by
compression molding at 200°C for 10 min.
While the unfilled PLA matrix displays an impact strength of 2.7 ± 0.1 kJ/m², the introduction of
P[CL-co-LA] copolyesters into PLA improves the impact strength of resulting materials,
reaching a maximum at 11.4 ± 0.3 kJ/m² for the experimental composition of 28 mol% LA.
However, out of this value, the improvement in toughness is less pronounced (Figure 2).
Figure 1. Photo of DSM
microcompounder 15 cc.
Study of the “composition-structure-properties” relationships
When toughness is considered, a better understanding of the resulting morphology must be achieved because of the great influence of morphological parameters [3, 5]. Accordingly, the
mean size and related size-distribution of the microdomains generated from these as-synthesized P[CL-co-LA] copolyesters dispersed throughout the PLA matrix were correlated to the
recorded impact strength values.
Mean size c
Width / Length
(nm / nm)
1 91 / 9 6.5 ± 0.6 30 / 30
2 72 / 28 11.4 ± 0.3 25 / 250-450
3 51 / 49 5.2 ± 0.3 ///
Table 2. Influence of the comonomer content on the
mean size of dispersed rubbery microdomains and
impact strength (E.I.) of PLA-based materials
containing 10 wt% of P[CL-co-LA] copolyester.
a) Experimental molar composition of the resulting
copolyesters as determined by 1H NMR.
b) Determined by Notched Izod impact tests according
to ASTM D256.
c) Determined by AFM.
As shown in Table 2, there is an optimum at 11.4 kJ/m2 obtained with the P[CL-co-LA] copolyesters containing 28 mol% in LA on the impact strength of resulting PLA-based materials.
AFM analyses provided some key-information with respect to the morphologies of resulting PLA materials (Figure 3). Whereas PLA-based materials with the best value in toughness show
fibrils regularly dispersed within the matrix, nodular morphologies are observed out of this maximum. For nodular morphologies, a gradual disappearance of the spherical nodules is
observed depending on the LA comonomer content, indicating that these copolymers are at least partially miscible with PLA matrix and induce a significant reduction in toughness.
Figure 3. AFM analysis of PLA-based material containing 10% weight of P[CL-co-LA] with various monomers feed ratios (molar composition CL/LA mol%: 91/9 in right, 72/28 in
middle and 51/49 in left).
Figure 2. Influence of the comonomer content on the impact strength of PLA-based
materials containing 10 wt% of P[CL-co-LA] copolyester.
1 2 3